of 21

• date post

15-Jul-2020
• Category

## Documents

• view

4
• download

0

Embed Size (px)

### Transcript of Plasticity in FEniCS - Katedra ... Plasticity Introduction Computational Methods Fluid Model of...

• Plasticity in FEniCS

Piotr Minakowski

Institute of Applied Mathematics and Mechanics, University of Warsaw E-mail: minak@mimuw.edu.pl

Mathematical Institute, Charles University E-mail: minak@karlin.mff.cuni.cz

SEMINÁŘ O SOFTWARU PRO GEOFYZIKY aneb Jednooćı slepým

• Outline

Plasticity Introduction Computational Methods

Fluid Model of Crystal Plasticity Motivations Model

Kirchhoff stress Numerical treatment

Implementation in FEniCS

• Motivations

Severe plastic deformation:

I large proportion of shear during deformation

I large strains (torsion experiment with multiple rotations)

I no major changes of shape and cross section

I changes of internal properties by grain refinement (UFG)

HPT / ECAE

• Aims:

I formulate flow model of crystal plasticity (Eulerian coordinates)

I provide consistent thermodynamic description

I observe formation of shear bands, reach steady state micro-structure

I validate by comparison with experimental data

ECAE HPT

• Large-deformation plasticity

Kröner decomposition

F = FeFp

I Fe, the elastic distortion, stretch and rotation of the lattice

I Fp, the plastic distortion distortion of the lattice due to formation of dislocations

F

Fp Fe

reference configuration

natural configuration

current configuration

. X . x = χ(X,t)

• The velocity gradient

In the virtue of Kröner decomposition

∇v = ḞF−1 = Ḟe(Fe)−1 + Fe(Ḟp ( Fp)

−1) (Fe)−1. Let us denote by Le and Lp elastic and plastic parts of velocity gradient (also called distortion-rate tensors)

Le = ḞeFe −1, Lp = Ḟp(Fp)

−1.

We have the decomposition

∇v = Le + FeLp(Fe)−1.

Moreover all the volumetric changes are assumed to result from elastic stretches in the lattice,

det Fp = 1, det F = det Fe > 0.

• Cauchy stress

Balance equation

Cauchy stress tensor T is divergence free

divT = 0

Jaumann rate of the Cauchy stress T

Ṫ + div vT−WT + TW = C : De where D = sym(L), W = skew(L) and C is fourth order spatial elastic tensor

C : D = λ(trD)I + 2µD.

where λ and µ are Lame coefficients.

D. Peirce, R.J. Asaro, and A. Needleman. Material rate dependence and localized deformation in crystalline solids. Acta Metallurgica, 31(12):1951–1976, 1983

• Resolved shear stress and slip systems

We define, resolved shear stress, the shear component of an applied stress resolved along a slip plane

τ (i) = s(i) · Tm(i) = T : s(i) ⊗m(i).

• Crystal plasticity assumption

Lp = N∑ i=1

ν(i)s (i) 0 ⊗m

(i) 0 ,

Dp = N∑ i=1

ν(i)sym (

s (i) 0 ⊗m

(i) 0

) s(1)m(1)

m(2)

s(2) m(3)

s(3)

To complete the system, slip rates ν(i) and hardening have to be specified,

ν(i) = ν0sgn (τ (i))

( |τ (i)| τ

(i) c

)1/m ,

τ̇c (i) =

∑ j

Hij |ν(j)|.

The second law of thermodynamics is satisfied

ξ = T : Dp = ∑ i

ν(i)T : (

s(i) ⊗m(i) )

= N∑ i=1

ν(i)τ (i) = ∑ i

ν0|τ (i)| ( |τ (i)| τ

(i) c

) 1 m

• Evolution of slip systems I Slip systems are changing with elastic stretches and rotations

s(i) = Fes (i) 0 and Ḟe =

( ∇v −

∑ i

ν(i)s(i) ⊗m(i) )

Fe.

I Evolution of slip directions

˙s(i) =

( ∇v −

∑ i

ν(i)s(i) ⊗m(i) )

s(i).

I We reformulate vectorial equations in therms of scalar unknowns (φ, s1, m1, s2, m2, s3, m3),

s(i) = si (cosϕi , sinϕi ), m (i) = mi (− sinϕi , cosϕi ).

ϕ̇ = (− sinϕ, cosϕ)T ( ∇v −

3∑ i=1

ν(i)s(i) ⊗m(i) ) s2(cosϕ, sinϕ),

ṡi = (cosϕi , sinϕi ) T

( ∇v −

3∑ i=1

ν(i)s(i) ⊗m(i) ) si (cosϕi , sinϕi ),

ṁi = (− sinϕi , cosϕi )T ( ∇v −

3∑ i=1

ν(i)s(i) ⊗m(i) ) mi (− sinϕi , cosϕi ).

• Scaled model I The unknowns are: velocity v, Cauchy stress T, density % and slip

directions s(i),

%,t +div (%v) = 0,

R1%v̇ + divT = 0,

Ṫ + Tdiv v + WT− TW = %C(D−Dp),

ϕ̇ = (− sinϕ, cosϕ)T ( ∇v − R2

3∑ i=1

ν(i)s(i) ⊗m(i) ) s2(cosϕ, sinϕ)

I Characteristic values %0 = 3000 kg m3 , V = 10

−5 m s , L = 10

−2m, ν0 = 10

−3 1 s , Σ = 70MPa

R1 = %0V

2

LΣ ≈ 10−12,R2 =

Lν0 V

= 1

I Update of remaining variables

mi , si , τ (i) c

• The elastic predictor/plastic corrector

EA. de Souza Neto, D Perí, DRJ Owen, Computational Methods for Plasticity, Wiley 2008

• Numerical treatment

I In time: One step finite difference

I In space: FE I P1 − dis.: T, ν(i) I P2: v I P1: %, ϕ, si , mi

I Newton-Ralphson method, analytic jacobian by automatic differentiation (FEniCS)

I For now direct linear solver of the fully coupled discrete system

I Boundary conditions by Nitsche’s method (ZTn · n, v · n)Γ2 + (Tn · n, zv · n)Γ2 +

β h (v · n, zv · n)Γ2 with β = 10

Main obstacles proper finite elements, power law with large exponent, boundary conditions

• Discrete formulation

Vh = {vh ∈W 1,2(Ω;R2); v|Γ1 = (0,−1), v · n|Γ2 = 0, v|K ∈ P2(K) 2 ∀K ∈ Th},

Rh = {%h ∈W 1,2(Ω;R); %h|Γ1 = 1, %h|K ∈ P1(K) ∀K ∈ Th}, Th = {Th ∈W 1,2(Ω;R2×2sym ); Th|K ∈ P1(K)2×2 ∀K ∈ Th}, Nh = {νh ∈ L2(R); νh|1 ∈ P1(K) ∀K ∈ Th}, Ah = {ϕh ∈W 1,2(Ω;R); ϕh|Γ1 = 0, ϕh|K ∈ P1(K) ∀K ∈ Th}.

Find (vh, %h,Th, ν1h, ν2h, ν3h, ϕh) ∈ Vh × Rh × Th × Nh × Nh × Nh × Ah, s.t.

(%h,t , z%) + (vh∇%h, z%) + (%hdiv (vh), z%) = 0 ∀z% ∈ Rh0,

R1 (%hv̇h, zv) + (Th,∇(zv)) + (Thn · n, zv · n)Γ2 + β

h (vh · n, zv · n)Γ2 = 0 ∀zv ∈ Vh0,(

Ṫh + Thdiv vh + WhTh − ThWh,ZT ) − (%C(Dh −Dph),ZT) + (ZTn · n, vh · n)Γ2 = 0 ∀ZT ∈ Th,(

ν (i) h − sgn (Th : s

(i) h ⊗m

(i) h )

( |Th : s(i)h ⊗m

(i) h |

τ (i) c

)20 , zνi

) = 0 ∀zνi ∈ Nh and i ∈ {1, 2, 3},(

ϕ̇h − (− sinϕh, cosϕh)T ( ∇vh − R2

3∑ i=1

ν (i) h s

(i) h ⊗m

(i) h

) s2h(cosϕh, sinϕh), zϕ

) = 0 zϕ ∈ Ah,

(1)

• Let’s dive into code

• Summary

Conclusions

I Eulerian formulation of crystal plasticity for large strain problems

I Consistent thermodynamic derivation of the model

I Finite element discretization method for fully coupled problem

I Numerical tools available to solve such systems

Further investigation

I adaptivity (time, space)

I stability conditions

I pass to rate independent (perfect plastic) limit

I mathematical properties (sequential stability result)

I ...

• Thank you for your attention.